silver and copper. The less pure gilding, which is thicker, can be considered a later repair, as the thinner, purer inlay adheres better to the silver. The adherence of the overall gold is quite poor. The lack of mercury from the gold analysis suggests that a fire-gilding technique was not used on the Gundestrup cauldron. The gilding appears to have instead been made by mechanical means, which explains the function of closely spaced punch marks on the gilded areas. An examination of lead isotopes similar to the one used on the silver was employed for the tin. All of the samples of tin soldering are consistent in lead-isotope composition with ingots from Cornwall in western Britain. The tin used for soldering the plates and bowl together, as well as the glass eyes, is very uniform in its high purity. Finally, the glass inlays of the Gundestrup cauldron have been determined through the use of X-ray fluorescence radiation to be of a soda-lime type composition. The glass contained elements that can be attributed to calcareous sand and mineral soda, typical of the east coast of the Mediterranean region. The analyses also narrowed down the production time of the glass to between the second century BC and first century AD. Flow of raw material The workflow of the manufacturing process consisted of a few steps that required a great amount of skill. Batches of silver were melted in crucibles with the addition of copper for a subtler alloy. The melted silver was cast into flat ingots and hammered into intermediate plates. For the relief work, the sheet-silver was annealed to allow shapes to be beaten into high repoussé; these rough shapes were then filled with pitch from the back to make them firm enough for further detailing with punches and tracers. The pitch was melted out, areas of pattern were gilded, and the eyes of the larger figures were inlaid with glass. The plates were probably worked in a flat form and later bent into curves to solder them together. It is generally agreed that the Gundestrup cauldron was the work of multiple silversmiths. Using scanning electron microscopy, Benner Larson has identified 15 different punches used on the plates, falling into three distinct tool sets. No individual plate has marks from more than one of these groups, and this fits with previous attempts at stylistic attribution, which identify at least three different